|Ask the Experts|
August 6, 2018
Cold Solder Joints on 0603 Components
We encountered cold solder joints on all of the 0603 components on the bottom side of a small batch of board assemblies, yet all the other larger components had good solder joints. These components are all near via holes, but this does not seem to be related to the cause. We replaced the solder paste on a new batch of assemblies, and the problem was eliminated. The solder paste used for the problem batch of assemblies had exceeded the 12 hour setup usage time we apply to solder pastes in our facilities by 1 hour. Was the problem likely due to the solder paste exceeding our 12 hour usage limit, or something else?
|Expert Panel Responses|
Technical Manager - Europe
In some cases, small solder deposits that look like cold solder could actually be graping, which looks very similar. Graping is a clumpy appearance on the outside of small solder deposits that forms because oxidized particles on the outside of the solder joint do not coalesce properly. Another clue is that larger components had good soldering, while smaller components didn't. Because of this, I would guess that what you experienced was actually this graping phenomenon, which could have been exacerbated by the exceeded usage limit as well. Leaving the paste out longer than usual could have contributed to excess oxide forming on the surface particles and inhibiting coalescence. In the future, to avoid this problem, limit the heat exposure for your assembly to minimize oxide formation and graping.
Technical Education Program Manager
IPC - Association Connecting Electronics Industries
Yes, We call it as Solder Paste Management, its an very important factor for Solder joints.
Bosch Automotive Electronics India Ltd.
It would seem that by exceeding the 12 hour setup usage time you changed the flux chemistry of your solder paste and created cold solder joints
Regional Sales Manager
OK International Inc.
I would of thought it could of been more like you have sheared thinned the paste too much especially if you over pressurise the squeegee with Lead Free in mind. Pressures of a maximum 1Kg per 50mm blade length for LEad Free should be used, nothing higher. If you over pressurise then you will have flux rich areas as well as flux starved which would definatley be more pronounced on smaller devices. Hence moving to fresher paste properly mixed has made a difference. Worth checking out and very simple to fix. I can't honestly believe by exceeding the meager 12 hour working life by one hour has made that much of a problem for you BUT it will have extended the over pressurising of the paste and subsequent the poor mix of flux contained within the flux Worth checking the print settings to confirm.
Technical Sales Manager
BLT Circuit Services Ltd
Since changing the used solder paste with fresh oneimproved the solder wetting results you can attribute the problems to thesolder paste condition. From my perspective the 12 hours exposure time for thesolder paste is excessive regardless of the conditions inside the printingmachine (temperature and humidity control) or the solder paste type andmanufacturer. Excessive exposure will create a good environment for oxidation.Since part of the solvents from the paste will evaporate, the smaller pads aregoing to be affected when it comes to proper reflow (the flux cannot beproperly activated anymore).
Engineering and Operations Management
|Submit A Comment|
Free Newsletter Subscription
Circuitnet is built for professionals who bear the responsibility of looking ahead, imagining the future, and preparing for it.
Insert Your Email Address